Spin glasses are systems whose magnetic moments freeze at low temperature into random orientations without long-range order1. It is generally accepted that both frustration and disorder are essential ingredients in all spin glasses, so it was surprising that PrAu2Si2, a stoichiometric compound with a well-ordered crystal structure, was reported2 to show spin-glass freezing. Here, we report on inelastic neutron scattering measurements of crystal-field excitations, which show that PrAu2Si2 has a singlet ground state and that the exchange coupling is very close to the critical value to induce magnetic order. We propose that spin-glass freezing results from dynamic fluctuations of the crystal-field levels that destabilize the induced moments and frustrate the development of long-range magnetic correlations. This novel mechanism for producing a frustrated ground state could provide a method of testing the concept of ‘avoided criticality’ in glassy systems.
Frustration arises from competing interactions that favour incompatible ground states1,3. For example, in rare-earth intermetallic compounds, the magnetic moments of the f electrons on each rare-earth site interact with neighbouring moments through Ruderman–Kittel–Kasuya–Yosida exchange interactions that oscillate in sign with increasing separation. Except for specific classes of geometrically frustrated lattices, well-ordered crystal structures produce either ferromagnetic or antiferromagnetic order, depending on the energy minimization of the interactions between all the neighbouring moments. However, when there is disorder, in either the site occupations or the exchange interactions, the additional randomness can prevent a unique ordered ground state. Instead, these systems may form spin glasses, which possess a multitude of possible disordered ground states, into one of which the system freezes below the glass transition temperature, Tg (ref. 1). In the thermodynamic limit, spin glasses show broken ergodicity, preventing significant fluctuations to any of the other degenerate spin configurations.
In recent years, two stoichiometric intermetallic compounds have shown evidence of spin-glass order, URh2Ge2 (ref. 4) and PrAu2Si2 (ref. 2), both nominally with the same tetragonal (ThCr2Si2-type) crystal structure. In both samples, classic spin-glass behaviour was observed (Tg=11 K and 3 K, respectively), with a frequency-dependent peak in the a.c. susceptibility and irreversibility in the field-cooled and zero-field-cooled magnetizations. It was quickly established that spin-glass freezing in the uranium compound resulted from site disorder on the rhodium and germanium sublattices. Extended annealing to remove this source of disorder was sufficient to transform samples into ordered antiferromagnets5. On the other hand, the spin-glass behaviour of PrAu2Si2 is very robust, and appears in the best-quality samples after extensive annealing. A recent Mössbauer study, combined with neutron and X-ray diffraction, concluded that interchange of gold and silicon atoms was less than 1% (ref. 6). Furthermore, the intentional introduction of disorder through the substitution of germanium for silicon stabilizes long-range antiferromagnetic order at concentrations greater than 12% (ref. 7). Finally, the praseodymium sublattice is face-centred tetragonal, and does not contain any of the triangular or tetrahedral motifs normally associated with geometric frustration3. This article seeks to explain the origin of magnetic frustration in PrAu2Si2, given that conventional models involving static disorder or lattice topology do not seem to apply.
First, it is essential to establish the nature of the praseodymium f-electron magnetism. The ninefold degeneracy of the 4f2-electron states is lifted by the crystal-field potential of tetragonal symmetry produced by the surrounding gold and silicon ions, giving a set of singlet and doublet levels. The doublet states have finite magnetic moments, but the singlet states are non-magnetic, except in the presence of exchange interactions with neighbouring sites as discussed below. Transitions between the crystal-field levels can be observed directly by neutron scattering as inelastic peaks, whose energies and intensities can be used to refine the parameters of the crystal-field potential. The peak widths are inversely proportional to the lifetimes of the excited states, which, in metals, are limited by conduction-electron scattering.
We have used neutron scattering to study samples of PrAu2(Si1−xGex)2, with x=0, 0.05, 0.10, 0.15, 0.20, 0.80 and 1, which were synthesized by arc melting followed by annealing in vacuum for four weeks at 850 ∘C. Neutron-diffraction measurements on PrAu2Si2 showed no evidence of any additional phases and measurements of the d.c. susceptibility in a field of 20 Oe showed the previously observed difference between field-cooled and zero-field-cooled susceptibilities, confirming a spin-glass freezing temperature of 3 K. The inelastic neutron scattering measurements were carried out at the Institut Laue–Langevin (Grenoble, France) on the high-resolution time-of-flight spectrometer IN6, using an incident energy of 3.1 meV, at temperatures ranging from 1.5 to 30 K.
In an earlier report, we determined the phenomenological parameters of the crystal-field potential in PrAu2Si2 (ref. 8) and showed that the ground state is a non-magnetic singlet with the first excited level a magnetic doublet at an energy Δ=0.7 meV (Fig. 1). The remaining levels are all above 7 meV, so this is effectively a two-level system at temperatures close to the glass transition.
Before discussing the origin of spin-glass behaviour, we review what is known about magnetic order in singlet ground-state systems. As the ground state of the isolated ion is non-magnetic, a magnetic moment can result only from an admixture of excited crystal-field states produced by exchange interactions with neighbouring praseodymium ions. There is a considerable body of research on such induced-moment systems, both theoretical9,10 and experimental11,12,13, showing that, for any given value of the low-lying crystal-field transition energy (Δ), there is a critical value of the exchange energy (Jex). Below this critical value, the system remains paramagnetic (that is, a Van Vleck paramagnet) at all temperatures. However, when the exchange is sufficiently strong, there is a critical temperature below which a ground-state moment forms spontaneously. In a two-level system, this temperature is given in a mean-field model by
where α is the dipole matrix element coupling the two levels and n is the degeneracy of the excited state. A calculation of Tc as a function of Jex for Δ=0.7 meV and n=2 is shown in Fig. 2.
In most induced-moment systems, Tc marks the transition to long-range order. Examples include Pr (ref. 12), Pr3Tl (ref. 11), Pr3In (ref. 14) and PrNi2Si2 (ref. 13). However, in the presence of static disorder, the low-temperature phase could also be a spin glass, as shown in ref. 15 in a mean-field model developed to explain scandium–terbium alloys16 and PrP0.9 (ref. 17). Sherrington15 calculated that a sufficiently large distribution of exchange interactions, δ Jex, could lead to spin-glass freezing. There is a multicritical point at
where z is the number of nearest neighbours. At larger values of δ Jex, spin-glass order would supersede long-range order. In the case of PrAu2Si2, for which z=4, δ Jex should be more than twice Jex, so Sherrington’s model requires a high degree of disorder to generate spin-glass behaviour.
Although such strong disorder seems unlikely in PrAu2Si2, we have explored the Sherrington model further by deliberately disordering the silicon sublattice through germanium substitution. It had already been found that long-range antiferromagnetism in PrAu2(Si1−xGex)2 is stabilized at concentrations x>0.12 (ref. 7). Our inelastic neutron scattering measurements show that the energy of the singlet–doublet transition is nearly independent of x (Fig. 3). What does change is the strength of the interionic exchange, Jex. In Fig. 2, we estimate the strength of Jex versus x, substituting the measured values of Tc in equation (1). This shows that Jex increases by a factor of four from x=0 to 1. Germanium doping should therefore be an ideal way of enhancing the exchange disorder that is central to the Sherrington model.
The most noticeable effect of chemical disorder is the large increase in the energy width of the singlet–doublet transition (Fig. 3). The peak lineshape is modelled by the convolution of a Lorentzian and a Gaussian function. The Lorentzian contribution arises from lifetime broadening, which will be discussed later. The Gaussian contribution arises from inhomogeneous broadening due to chemical disorder and the energy dispersion of the crystal-field excitations18. There is a small Gaussian contribution in PrAu2Ge2 (σ=0.13 meV) due to energy dispersion, but no Gaussian component is required to fit the data from PrAu2Si2, whereas the Lorentzian widths are very similar in the two compounds. As the exchange is estimated to be a factor of four smaller in the pure silicide, we believe that chemical disorder dominates the Gaussian contribution at low values of x.
If we convolve the peak lineshape with the instrumental resolution to produce the fits in Fig. 3, we estimate that the Gaussian width rises approximately linearly with x, for x≤0.2 (Fig. 4a). This shows that there is no correlation between the measured inhomogeneous broadening and the transition to long-range antiferromagnetic order and confirms that static disorder is not the critical factor determining the occurrence of spin-glass freezing.
If static disorder is not responsible for the frustrated ground state, we must seek an alternative explanation, one that should take into account the observation in Fig. 2 that spin-glass freezing occurs only in proximity to the induced-moment phase boundary. We propose that relaxational broadening of the singlet–doublet transition provides the key. Figure 4b shows the temperature dependency of the transition half-width in PrAu2Si2, which increases from about 0.13 meV at 1.6 K to 0.26 meV at 20 K. The data are consistent with standard models of f-electron relaxation due to fluctuations in the single-site crystal-field populations, which causes the rapid increase at low temperatures, and conduction-electron scattering19. The important result is that the width remains substantial down to the lowest temperature, with the full-width at half-maximum only falling to a value of 43% of the transition energy at the glass transition.
This energy broadening will play a significant role in disrupting induced-moment formation. Figure 5 shows the complementary phase diagram to Fig. 2, in which Jex is fixed to the estimated values in PrAu2Si2 and PrAu2Ge2 and Tc is plotted against Δ. The induced moments are predicted to be stable in both compounds; however, if we superimpose the broadened peaks, we see that the peak traverses the phase boundary significantly in the silicon compound but not in the germanium compound. Strictly speaking, the width is proportional to the inverse lifetime of the excited state and not the lifetime of the induced ground state; however, this makes it highly plausible that dynamic fluctuations would disrupt the stability of such moments in PrAu2Si2, but not in PrAu2Ge2.
In induced-moment systems, a precursor of long-range order is the appearance in neutron scattering of a quasielastic ‘central’ peak close to the wavevector of the ordered phase, which is caused by fluctuating regions of short-range magnetic order20. For example, in Pr3Tl, the correlation length associated with this central peak diverges as the critical temperature is approached21. Our conjecture is that any divergence of the magnetic correlation length in PrAu2Si2 is suppressed by dynamic fluctuations that limit the lifetime of induced moments and so introduce magnetic site and exchange disorder. This scenario is similar to the ‘avoided criticality’ discussed in the theory of structural glass transitions by Tarjus et al. 22. In their review, they argue that many glasses are close to a conventional second-order phase transition, but that frustration prevents the divergence of the correlation length. This would make the PrAu2(Si1−xGex)2 series promising candidates to test their scaling predictions because the degree of frustration can be tuned by varying Jex or Δ with dopant concentration or pressure.
There is considerable interest in the ways that spin systems respond to the presence of substantial frustration. Historically, this subject was stimulated by the observation of spin-glass freezing in disordered alloys and compounds, and has more recently focused on systems where the lattice geometry produces a macroscopic degeneracy of possible spin configurations. We suggest that PrAu2Si2 reveals a new avenue to achieving frustration in systems with neither static disorder nor geometrically frustrated lattices, through dynamic fluctuations, either thermal or quantum, in proximity to a critical phase boundary.
Fischer, K. H. & Hertz, J. A. Spin Glasses (Cambridge Univ. Press, Cambridge, 1991).
Krimmel, A. et al. Spin-glass behavior in PrAu2Si2 . Phys. Rev. B 59, R6604–R6607 (1999).
Ramirez, A. P. Geometric frustration: Magic moments. Nature 421, 483 (2003).
Süllow, S. et al. Spin glass behavior in URh2Ge2 . Phys. Rev. Lett. 78, 354–357 (1997).
Süllow, S. et al. Disorder to order transition in the magnetic and electronic properties of URh2Ge2 . Phys. Rev. B 61, 8878–8887 (2000).
Ryan, D. H. et al. Site disorder and spin-glass ordering in PrAu2Si2 . J. Appl. Phys. 97, 10A908 (2005).
Krimmel, A. et al. The evolution from long-range magnetic order to spin-glass behaviour in PrAu2(Si1−xGex)2 . J. Phys. Condens. Matter. 11, 6991–7003 (1999).
Goremychkin, E. A., Osborn, R., Rainford, B. D., Adroja, D. T. & Koza, M. Magnetic dynamics of the spin-glass system PrAu2Si2: An inelastic neutron scattering study. J. Magn. Magn. Mater. 310, 1535–1536 (2007).
Grover, B. Dynamical properties of induced-moment systems. Phys. Rev. 140, A1944–A1951 (1965).
Cooper, B. R. Magnetic excitons in real singlet-ground-state ferromagnets: Application to Pr3Tl and fcc Pr. Phys. Rev. B 6, 2730–2743 (1972).
Birgeneau, R. J., Als-Nielsen, J. & Bucher, E. Magnetic excitons in singlet-ground-state ferromagnets. Phys. Rev. Lett. 27, 1530–1533 (1971).
Houmann, J. G. et al. Magnetic excitations and magnetic ordering in praseodymium. Phys. Rev. Lett. 34, 587–590 (1975).
Blanco, J. A., Nicklow, R. M. & Schmitt, D. Paramagnetic excitations in singlet ground state PrNi2Si2 . Phys. Rev. B 56, 11666–11672 (1997).
Heiniger, F., Bucher, E., Maita, J. P. & Longinotti, L. D. Thermodynamic properties of superconductors containing impurities in a crystal-field singlet ground state. Phys. Rev. B 12, 1778–1789 (1975).
Sherrington, D. The induced-moment spin glass: Simple mean-field theory. J. Phys. C 12, L929–L933 (1979).
Sarkissian, B. V. B. & Coles, B. R. Spin-glass to Overhauser-alloy transitions in Yt–rare-earth and Sc–rare-earth alloys. Commun. Phys. 1, 17–23 (1976).
Yoshizawa, H., Shapiro, S. M., Hasanain, S. K. & Guertin, R. P. Neutron scattering study of the crystal electric field levels in an induced-moment spin-glass PrP0.9 . Phys. Rev. B 27, 448–455 (1983).
de Gennes, P. G. Inelastic magnetic scattering of neutrons at high temperatures. J. Phys. Chem. Solids 4, 223–226 (1958).
Jensen, J., McEwen, K. A. & Stirling, W. G. Magnetic excitations in the longitudinally polarized antiferromagnetic phase of praseodymium. Phys. Rev. B 35, 3327–3340 (1987).
Lindgård, P.-A. Correlation theory of planar magnets. Phys. Rev. Lett. 50, 690–693 (1983).
Als-Nielsen, J., Kjems, J. K., Buyers, W. J. L. & Birgeneau, R. J. Observation of a central mode in an exchange-coupled singlet-groundstate system. J. Phys. C 10, 2673–2678 (1977).
Tarjus, G., Kivelson, S. A., Nussinov, Z. & Vlot, P. The frustration-based approach of supercooled liquids and the glass transition: A review and critical assessment. J. Phys. Condens. Matter 17, R1143–R1182 (2005).
We thank A. Murani and R. Stewart for scientific discussions and assistance with the ILL experiments. This work was supported by the US Department of Energy Office of Science, under contract No DE-AC02-06CH11357. R.T.M. is also supported by Research Enhancement Development at UNC.
About this article
Cite this article
Goremychkin, E., Osborn, R., Rainford, B. et al. Spin-glass order induced by dynamic frustration. Nature Phys 4, 766–770 (2008). https://doi.org/10.1038/nphys1028
Physical Review Research (2021)
Scientific Reports (2021)
ACS Omega (2020)
Physica B: Condensed Matter (2020)
Scientific Reports (2020)